Compressive Strength test results of cement, which is milled by the complex «Activator С500».Portland Cement Compressive Strength Specifications in MPa and mesh analisys. 
№  Cement  Cement input  Cement stored in 24 hours  Cement stored at 2 weeks  Growth of cement strength after grinding  Cement strength loss after stored for 2 weeks  Mesh analisys of milling cement 
Compressive strength at 4 weeks, Mpa 
1  Cement CEM II 32,5N  41,2  54,9  53,0  35%  3%  4%>80μ; 96%<80μ 
2  Cement CEM I 42,5N stored for 1,5 years.  40,2  59,8  58,8  50%  2%  7%>80μ; 93%<80μ 
3  Clinker, Iskitimcement factory    47,1  47,1    0%  8%>80μ; 92%<80μ 
4  Cement blend (1): CEM I 42,5N + fly ash 50% : 50%    41,2  35,3    10%  8%>80μ; 92%<80μ 
5  Cement blend (2): CEM I 42,5N + ground granulated slag 50% : 50%    35,3  34,3    2%  11%>80μ; 89%<80μ 
6  Cement blend (3): CEM I 42,5N + ground granulated slag precursory milling 50% : 50%    49,0  49,0    0%  3%>80μ; 97%<80μ 

Compressive Strength Specifications of Cements is measured on GOST of Russia 310.481. 
The table shows the results of the activation of cement  cement №1 and №2. Compressive Strength of PC CEM II 32,5N (cement №1 in table) before milling was 41,2 Mpa. After activation (milling) compressive strength of the PC is already 54,9 Mpa. Thus, the increase in strength at milling is 35%. 
PC CEM I 42,5N (cement №2 in table) has lost compressive strength when stored for 1,5 years, which was 40,2 Mpa. After milling (activation) the compressive strength of the cement is already reached 59,8 Mpa. Thus, the increase in strength at milling is 50%. 
Also, the table shows the results of comilling of cement mixtures, consisting of cement in Table №3 with fly ash (a mixture of cement 1) and with ground granulated slag (cement mixture of 2 and 3). 